J. L. Gale and D. A. Dixon, Phys. Rev. B, 57, 12002. (1998). 27. A. J. Stecki, J. Xu, H. C. Mogul, and S. M. Prokes,. J. Electrochem. Soc., 142, L69 (1995). 28.
J. Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemical Society, Inc.
7. 5. R. Kasi, M. Liehr, P. A. Thiry, H. Dallaporta, and M. Offenberg, Appl. Phys. Lett., 59, 108 (1991).
8. K. Saga and T. Hattori, Appi. Phys. Lett., 71, 3670 (1997).
9. K. Saga and T. Hattori, J. Elect rochem. Soc., 144, L253
10. K. Saga and T. Hattori, J. Electrochem. Soc., 144, L250 (1997).
11. T. Ohmi, T. Imaoka, T. Kezuka, J. Takano, and M. Kogure, J. Electrochem. Soc., 140, 811 (1993).
12. N. Miki and T. Ohmi, in Ultra Clean Technology, 9, Suppi. 2 (1997).
On the Correlation of Aqueous and Nonaqueous In Situ and Ex Situ Photoluminescent Emissions from Porous Silicon Evidence for Surface-Bound Emitters James 1. Goe, Frank P. Dudel, and Lenwarci Seals
School of Physics, Georgia Institute of Technology, Atlanta, Georgia 30332-0430, USA Melissa Reger
School of Chemwal Engrneering and Materials Science, Sarkeys Energy Center University of Oklahoma, Norman, Oklahoma 73019-0628, USA
Paul Kohl* School of Chemical Engineering, Georgia Institute of Technology, Atlanta, Georgia 30332-0100, USA
Lawrence A. Botfomley* School of Chemistry and Biochemistry, Georgia Institute of Technology, Atlanta, Georgia 30332-0400, USA
Porous silicon samples were prepared by anodizing p-doped Si(100) substrates in both aqueous (HF/H20, HF/CHOH, HF/CH3OH/H20, HF/C2H5OH/H20) and nonaqueous (MeCN/HF) media. The time-dependent porous silicon photoluminescence (PL) was monitored during the etch (in situ) and after removal from the etch solution (ex situ). Correlation of the ex situ and in situ PL indicates that the composition of the etchant solution plays an extremely important role in the onset, time-dependent intensity, and lifetime of the emission, both in and out of solution. The effect of etchant solution additives (ethylene glycol, CH3OH, C2H5OH, NaF, HC1, and NaC1) on the porous silicon PL both during arid following the
etching cycle, was also determined. The distinct and different correlations found between aqueous and nonaqueous etchants provide insights into the mechanism of PL. These results, when considered in the context of quantum chemical modeling, strongly suggest surface-bound silicon oxyhydride moieties as the source of the porous silicon PL. Introduction The visible photoluminescence (PL) extending from 500
to 800 nm which characterizes electrochemically (EC) produced porous silicon (PS)12 at room temperature has been the subject of considerable interest because of its potential use in the development of silicon-based optoelectronics, displays, and sensors. While this luminescence is thought to occur near the PS surface,34 the source of this visible emission is controversial as the efficiency and wavelength range of the emitted light can be affected by the physical
and electronic structure of the surface, the nature of the etching solution,56 and the nature of the environment into which the etched sample is placed.9 With this parameter dependence, it is surprising that, with few exceptions1011 PL spectra are generally reported for PS samples (formed in dilute HF solutions) which have already been dried in air or more inert environments after undergoing etch and rinse treatments. These ex situ samples provide spectral information but do not indicate the evolution of the PS luminescence. It is therefore of interest to observe the PL as it evolves, in situ, during the etching process and fol— lowing, while the sample is still wet by the etching solution or has been treated by an appropriate rinse. Here we examine the in situ development of the PS photolumines— cence in several etch solution environments as well as the controlled modification of these environments. For certain *
Electrochemical Society Active Member.
select environments, we also consider the net effect of these in situ treatments on ex situ behavior.
We have carried out an extensive series of experi—
ments5'79'12 in both aqueous (HF/H20, HF/CHOH, HF! CH3OH/HZO, HF/C2H5OH/H20) and nonaqueous (MeCNf HF, anhydrous) etching media. We monitor the time-depen-dent PL, in situ, during the etching cycle and before the PS
sample is removed from the etching solution, including a study of the effect of the additives ethylene glycol, CH3OH, C2H5OH, NaF, HC1, and NaCI on the in situ luminescence process. We also consider the effect of these treatments on the ex situ behavior of the PL after removal of the PS from
the etching solution. By correlating the ex situ with the in
situ behavior of the PS, we find that the aqueous electrolyte composition plays an extremely important role in
the onset, time-dependent intensity, and lifetime (solution) of the PL emitters.7-912 Comparable studies on nonaqueous electrolytes are found to demonstrate distinctly different correlations between the in situ and ex situ behavior and we use these resuilts to provide possible insights into the mechanism of the PL process. Further, in complement to the experimental studies, we introduce a quantum chemical modeling which suggests that silicon oxyhydride-like
fluorophors9 strongly bound to the PS surface are the
source of the PS PL. The silicon oxyhydride moiety can be viewed as a highly reactive intermediate in the oxidative pathway between the hydrophobic Si—H surface generated in the HF etching process and the hydrophilic Si02 surface.
.1 Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemical Society, Inc.
The studies reported here complement those of Sailor et al.'3-'6 We consider that the oxyhydride fluorophors are
The results of our experiments conducted in aqueous and nonaqueous media provide support for a surface-
bound to the PS surface and that they are to be distinguished from surface adsorbates. Sailor et al.'" have
bound molecule-like emitter as the source of the FL from
reported the hole transfer quenching of the PL from PS by ferrocene'3 and the irreversible quenching due to aromatic hydrocarbons and redox active solutes,"3 they have also demonstrated the reversible quenching of the PS lumines-
including the early appearance in time (% C/)
30 40 50 60
.-ci)C ' '
6500 '7000 Wavelength (Angstroms)
( OO 10 20
20%HF in MeOH
Fig. 3. P1 spectra (ex situ) for PS samples excited by a nitrogen laser and prepared by etching Si(100) at 4 mA/cm2 for approximately 10 mm in (a) 20% HF in H20, (b) 20% HF in MeOH, (c) anhydrous MeCN/HF, and (d) 50% HF in MeOH. The prepared samples were rinsed in MeOH and dried in air for several minutes before the P1 was taken. The spectra taken at a time gate of 0.8—100 ps have been corrected for system response.
is first wet by the etching solution through the
commencement of the etch cycle.
Monitoring of "green and orange-red" photoluminescent emissions—To study the evolution of the PS PL, the emis-
sion is monitored in situ at two wavelengths, 5200 and 6200 A. The 6200 A wavelength represents the best combi-
nation of the peak PL wavelength, convolved with the spectrometer + phototube system response, which can be used to monitor the orange-red PL emission commonly characterizing UV-pumped (? < 350 nm) porous silicon. 5200 A represents the wavelength of choice5 to monitor the PL precursor state, whose signature has been observed by a more limited group of researchers, as it is characterized by a green spectral emission which appears to transform in time to the final orange-red emitter.5 Figure 4 demonstrates the PL at these two wavelengths where Si(100) is etched in each of the four basic etching solutions considered in this study.
Anhydrous HF/MeCN Etch—The data for the nearly anhydrous 2 M HF in MeCN etch solution depicted in Fig. 4a at higher resolution'2 shows that the 6200 A PL is observed as early as 10 s into the etching process, long before pores can be formed. Figure 4a indicates that the 6200 A PL rises linearly during the etching process followed by a sharp rise in the PL intensity after the EC etch-
ing cycle is terminated. At the sensitivity of the detector used in this study and for the extremely low water content present, during the etch cycle, little or no detectable PL was observed at 5200 A until after the etching current was terminated. Here, similarly, a significant rise in PL intensity was observed at 5200 A. A gradual decay in the PL was then observed at each wavelength while the silicon remained in solution. This basic behavior was obtained for several etch currents ranging from 4 to 24 mA/cm2; however, it was clear that the slope of the initial linear rise in PL emission intensity decreased with increasing etch current over this range.7 This dependence, depicted for 11 and 24 mA/cm2 etching currents in Fig. 5a, in concert with the
sharp rise in PL intensity after the etching current is terminated, suggests that the etching process both creates and destroys the PL emitters. This important interplay,7
10 20 30 40 50 60 Time (Minutes) Fig. 4. P1 intensity (arbitrary units) at 5200 and 6200 A vs. time for Si(100) etched at4 mA/cm2 in (a) 2 mol/1 HF MeCN for 10 mm (this P1 onsets within lOs), (b) 6 mol/1 HF in H20 (20% HF in H20)
for 12 mm (this Pt onsets within 7600 A are significant. The time gate for sampling was 0.8—100 p.s.
J. Electrochem. Soc., Vol. 145, No.9, September 1998 The Electrochemical Society, Inc.
depicts the time dependence of the PL at 6200 A for a pSi(100) wafer etched in 14 mol/L HF in MeOH. No PL was observed during the etching process. After the etch was terrnrnated, a gestation period of approximately 24 mm pro-
PL at 6200 Angstroms with continuous etching
ceeded the observation of any visible PL. Clearly, the surface of the PS is undergoing significant chemical changes during this extended time period to produce the luminescence.
in situ PL spectra as a function of etch solution.— Photoluminescent spectra from PS, formed and allowed to
remain in the etching solution for limited periods, are depicted in Figure 10. For the three solutions considered, the silicon was etched for 12 mm at 8 mA/cm2. The PL data were recorded while the samples remained in solution, 2—3 mm after the etching current was terminated for those samples placed in a near-anhydrous MeCN/HF solution and in a 20% HF in MeOH solution and —24 mm after
termination for the 50% HF in methanol solution. The
ratio of the PL at 6200 A to that at 5200 A for the MeCN/HF etching solution can be clearly assessed from Fig. 10. These spectra, obtained for the wetted PS samples, are clearly blue-shifted relative to the spectra depicted in Fig. 3 and obtained for similarly prepared PS samples dried in air. In other words, the drying of the PS sample caused the peak spectral emission wavelength to shift by several hundred angstroms to longer wavelengths for each of the basic solutions used in this study The red shift in the PL emission with increased exposure to air must be intimately tied to the transformation of the emitting mediurn on the PS surface.
10 mA/cm2 (4
150 180 210
Time (Minutes) Fig. 11. P1 emission intensity as a function of etch current and time for the etching of Si( 100) in a 6 M HF/H20 solution at the indicated etch currents.
Effect of etch current density—Figure 11 exemplifies the effect of etch current density on the PL observed during the
etch cycle. Here the silicon was etched in a 6 M HF/H20 solution at a current density of 10 mA/cm2 for 70 mm. The 6200 A PL clearly increased in intensity during the etching
PS—Post etch treatments.—The varied nature of the in situ
process. As the current density was increased to 16 mA/cm2, a sudden increase in the 6200 A PL was observed, followed
by a continuous albeit less pronounced increase in the PL intensity with etch time over the next 60 mm. 'When the etch
current was increased to 30 mA/cm2, the PL intensity increased quickly followed by a rapid decay over the next 70 mm, suggesting the onset of electropolishing. A similar
although at slightly higher etching currents, is
also observed for the 6 M HF/H20/MeOH solution.
The influence of additives on the in situ PL from PL characteristic of the basic etching solutions which we have outlined has also focused our attention on the effect of additives to the etching solution and hence on post-EC etch treatments. The stabilizing effect of small quantities of water on the anhydrous etching process,7 as well as the effect of ethylene glycol5 on the green and orange-red PL from a sample etched in HF/H20 and HF/H,O/CH;3OH solutions are exemplary. We have found that samples prepared in any of the four basic etching solutions, once cleaned in a combination of
doubly deionized water and methanol or ethanol and
allowed to dry, yield a significant ex situ PL. If a cleaned sample is immediately placed in doubly deionized water, we observe a slow rise in the in situ PL intensity at both 5200 and 6200 A. Similarly, if such a cleaned sample is placed in an ultrahigh-purity methanol or ethanol solution, the in situ PL slowly increases and gradually dimin-
ishes on the time scale of several hours. However, this behavior is in sharp contrast to the effect of immersing the PS in a combination of the alcohols with HE b
Wavelength (Angstroms) In Situ P1 observed after etching fri aJ 50%HF ri MeOH, b) MeCN /HF, and c) 20%HF in MeOH
Fig. 10. Pt. spectra (in situ) For porous silicon exdteci by a nitro-
gen laser after etching Si(100) for 12 mm at 8 mA/cm2 in (a) 14 mol/L HF in MeOH(aq) (50% HF in MeOH); (b) near-anhydrous
2 M I-IF in MeCt.1; and (c) 6 md/I HF in MeOH(aq) (20% HF in MeOH). These in situ spectra taken at a time gate for sampling of 0.8—100 p.s should be compared with the ex situ spectra in Fig. 3.
Post etch treatment with ethanol—The PL induced by an aqueous HF etch [e.g., HF (20%) in H2OJ can be readily depressed through the postetch addition of ethanol to this solution. The 6200 A PL is most affected, showing a definite decay upon addition of ethanol to the etch solution. However, after displaying an initial dip in intensity, the 5200 A PL is observed to recover to virtually its initial level. The effect of ethanol can, however, be more diverse. We exemplify with the results for a silicon sample first etched in a solution of 20% HF in water for 10 mm i oltowed by a subsequent etch after the addition of ethanol to this solution. The 6200 A PL intensity in the HF/H20 solution increased after the etch was terminated as exemplified in Fig. 4b. Depicted in Fig. 12 is the 6200 A PL as a function of time when 700 pL of ethanol was added to 2 mL of the 20% HF/H20 etching solution and this solution was used to etch the silicon sample for a second time. Although the 6200 A PL increases more rapidly during the etch period, after the cessation of the EC etch, the PL intensity decreases much more rapidly and is almost completely
J. Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemical Society, Inc.
HF in H20 with 700.tl EtOH added
20% HF in H20
Fig. 12. Pt emission as a function of time showing the effect of adding ethanol to a 20% HF/H20 etching solution. Here 700 p.1 of EtCH was added to 2 ml of the HF/H20 solution previously used to etch a Si(100) sample and the subsequent sqlution was used to etch the silicon again. We compare the 6200 A Pt emission intensity to that depicted in Fig. 4b.
quenched within 30 mm. This behavior, while not as pro-
nounced, closely parallels that observed for a silicon wafer initially placed in an HF/H20/MeOH solution (Fig. 4c).
Postetch treatment with methanol—Figure 13 demonstrates the diverse quenching effect which the simple alcohols can have on the PS PL. The data depicted in the figure were obtained using a concentrated HF (48%) etch upon the addition of methanol. A PS sample was produced from a 14 M HFJH2O solution etched for 12 mm at a current density of 8 mA/cm2. The PL decay was then monitored after the EC etching process was complete and while the PS sample
remained in the etching solution. After approximately
50 mm of exposure to the HF solution, 100 p.L of methanol was added to 2 mL of the concentrated HF solution and an
immediate loss (Fig. 13) in PL (6200 A) intensity was
observed. At approximately 68 mm after the termination of the EC etch, a second 500 jiL aliquot of methanol was added to the etching solution and an extremely rapid quenching of the PL was observed. At 5200 A, a similar albeit somewhat slower quenching was monitored.
It is important to emphasize that if we allow a PS sample to remain in the HF/H20/MeOH etching solution after the EC etching cycle is complete, the PL will be quenched completely within 15 mm. We find that the quenching cycle appears to follow the reverse of the development of the PL (Fig. 4) as the orange-red PL quenches much more rapidly than the green PL. Only after the orange-red PL is completely quenched do we observe the complete quenching of the green FL5 in an HF/MeOH-based solution. We have also observed PL from an HC1/H20 solution following an etch cycle. In sharp contrast, the addition of methanol to this HC1/H20 etching solution does not appear to quench the FL but may in fact provide some enhancement. In further contrast, we find that a strongly photolummnescent sample cleaned of HF and placed in MeOH will exhibit a signif icant FL for several days. If we add a single drop of HF
etching solution to a previously etched PS sample as it
soaks in MeOH, the PL is rapidly quenched. The results in
an HF/MeOH environment, obtained when methanol is introduced into an aqueous HF etching environment or vice versa, are to be contrasted with a virtually complete lack of quenching when MeOH is introduced into a nonaqueous HF/MeCN etching solution. It seems apparent that
the interaction between methanol and to a lesser extent ethanol and HF in an aqueous solution leads either to the
formation of a solution phase compound which very effectively quenches the triplet exciton excited state giving rise to the PL from PS or accelerates the PS surface oxidation or dissolution process.
Postetch treatment of PS samples in methanol, H20— NaF.—The importance of fluoride ion to the dissolution process is clearly outlined in Fig. 14. Here we indicate the effect of the introduction of NaF prepared in a saturated methanol solution (—0.4 M), to PS samples photoluminescing in air and a methanol solution. As Fig. 14a and b indicate, the postetch FL from a porous silicon sample placed in methanol solution increases somewhat more rapidily than does that for a sample placed in air. The introduction of NaF immediately quenches this FL on a time scale of seconds. Fluoride ion is clearly a very effective quencher. The consideration of diffusion effects in the etching solution suggests that the quenching process results from the extremely rapid dissolution of the top few surface layers which contain surface-bound emitters. Post etch treatment with HC1—PL enhancement and stabi-
PL at 6200 Angstroms
0 0 -c
lization—Figure 15 depicts the in situ effect of water and HC1 on the orange-red PL from a PS sample previously dried in air. The PS sample was first etched in a methanol! 20% HF [6 mol/L HF in MeOH(aq)] solution for 10 mm, washed with methanol, dried in air, and then placed first in a solution of doubly deionized water and then —6 M HC1. The intensity of the FL increased somewhat upon removal from the HF solution and again increased more rapidly as the sample was placed in water.78 However, after adding HC1,78 the orange-red FL intensity increased significantly (Fig. 15) and remained virtually constant over the period (up to 3.5 h) in which the sample was present in the HC1 solution. Within the time frame of these described processes, the wavelength-dependent spectral profile of the PL emission spectrum was only slightly altered from the time it
was removed from the HF etching solution and dried through the period in which the sample remained in the HC1
solution. The introduction of HC1 clearly has a profound stabilizing effect on the in situ PS FL.
We have also examined the influence of the heavier 60
Minutes in 48% HF Fig. 13. Plot of 6200 A Pt intensity as a function of time when methanol is added too sample prepared by etching silicon (100) in a concenfrated HF solution. The methanol enhanced decay of the emission is apparent. See text for discussion.
acids HBr and HI on the nitrogen laser excited FL from a PS surface.8 In contrast to the apparent stabilizing effect of hydrochloric acid on a PS surface photoluminescing in doubly deionized water, HI almost completely quenches the PL. The effect of an HBr solution is intermediate. We have also examined the effect of HC1 introduction into an HF/H20 etching sOlution in the early stages following the etching process. Again, the enhancement and
stabilization of the 6200 A orange-red PL is apparent; however, we find that the effect of HC1 on the 5200 A flu-
1 Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemica! Society, Inc.
3000 Plcl,ed in 20%
I-I Fi MeOH
Add NaF(MeOH (5.5g NaE/3Dcc MeOH)
Sample placed in MeOH
Fig. 14. Effect of introducing NaF (fluoride) to the PS etch solution (a, left) for o sample etched in 6 M HF in MeOH(aq), rinsed in methanol, and dried in air for - 12 mm and then placed in a saturated NaF/MeOH solution, and (b, right) for a sample etched in 6 M HF in MeOH(aq),
placed in air for 10 mm and then in methanol for —90 mm, followed by addition of NaF. P1 intensity increases after removal from the HF/MeOH etch solution in either air or methanol and is quenched immediately upon introduction of fluoride ion.
orescence, which rises much more slowly, is far less pro-
nounced. HC1 appears to preferentially stabilize the
orange-red emitter. Postetch treatment of PS samples in methanol—NaCI.— The intriguing stabilization of the PS FL in an HO solution focuses our attention on the effect which chloride ion
has on the FL process. As the data in Fig. l6a and b
demonstrate, a stabilization of the PL emission rate from
an etched PS surface, albeit at a notably lower photon
count, accompanies the addition of NaC1 to a luminescing PS sample. In fact, an intriguing behavior is monitored. As we have noted, in the absence of Mad, the 6200 A PL from PS placed in a methanol solution slowly rises, eventually peaks, and then more gradually decreases in intensity. If NaC1 is added to this solution before the FL has reached its maximum intensity in methanol, the PL slowly increases to a maximum intensity and then plateaus. As Fig. iSa demonstrates for a PS sample introduced to a NaC1-saturated solution in methanol, this plateau is reached over a time scale of several hours (compared to 30 mm for HC1). If, however, the saturated NaCl solution is introduced to a
scales linearly with incident laser photon flux, demonstrating that the observed behavior does not result from multiphoton processes. Finally, we observe that the ex situ FL spectrum in air, in time will generally equalize regardless of
Equal volume of HCI added to water 20000 U)
how the sample is prepared. The ex situ PL gradually
increases in intensity over the course of several hours and then plateaus in intensity as the spectrum red shifts.
C 0 4-
Trends in ex situ PL spectra.—From the data in Fig. 3 and 9, it should be clear that the ax situ PL spectra (i) red shift in air relative to the observed in situ luminescence and (ii) red shift with the duration of the overall etching process and are affected by a previous etch cycle. We observe that a sample, prepared in a near-anhydrous in situ environment (MeCN/HF), after it is washed (methanol), dried, and placed in air, displays a considerably weaker initial luminescence than does a sample prepared in an aqueous HF solution (20% HF/H20, 20% HF/MeOH). Samples prepared in aqueous HF generally display a clear luminescence immediately after ex situ preparation [washing (methanol), drying in airl. With time, however, the PL from the sample generated in the anhydrous MeCN/HF increases and may eventually surpass that from the sample generated in aqueous etch. In fact, the most intense ex situ PL which we have observed
results after etching in a near-anhydrous solution. The ex situ spectra which we have observed do not appear to shift with increasing laser power. In fact, their intensity
Effect of Water and HCI on 620 nm PL
methanol solution in which the PS sample is previously placed, as indicated in Fig. 16b, after the PL has peaked in the methanol solution, the PL is stabilized at an intensity corresponding closely to that at the time of the NaCl introduction. This is certainly an intriguing result which portends means to stabilize the PL from porous silicon with appropriate chloride solutions.
Discussion have characterized several environments in which FL can be generated on an etched PS surface and have established conditions under which this FL can be stabilized, enhanced, or quenched. The experimental results which we have outlined are summarized in Table I. We argue in this discussion that the origin of the visible FL emission from PS is reasonably associated with a surfacebound chemical entity and that the emission correlates with a transition originating from a triplet exciton, as We
Time (Hours) Fig. 15. The effect of an HCl solution on the stabilization of the PS P1 for a sample previously dried in oir and placed in doubly deion-
ized water. The wavelength monitored was 620 nm and the data were taken using nitrogen laser excitation. Here the Pt rises slowly in air and water and then increases precipitously in HCl solution.
established by Stutzmann and co-workers.2320 We suggest
that this surface-bound source can be viewed as a
silanone-based silicon oxyhydride emitter bound to the PS surface. In this discussion, we evaluate the formation of the photoluminescent sources and their subsequent loss by
either their oxidation to Si02 or dissolution in the HFbased etching solutions investigated in this study.
J. Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemical Society, Inc. 8000
620 nm P1 in NaCI Solution
Etched sample in MeOH
Fig. 16. Effect of NaCI introduction on a luminescig PS sample in methanol. (a, left) The NaCI prepared as a saturated solution (—0.2 M) is added to a sample photoluminescing at 6200 A in MeOH before the PL has reached its peak intensity. The solution stabilizes at the peak PL intensity although at a much longer time scale than,that for HCI (Fig. 15). (b, right) The NaCI prepared as a saturated solution (0.2 M) is added to a sample photoluminescing in MeOH (6200 A) after the Pt intensity in methanol has peaked. The solution is stabilized at the intensity upon addition.
It has been established that PS is formed by an oxidation-dissolution mechanism where silicon oxides, current
density, and crystallographic structure play a pivotal
role231 and the rate of growth of the oxides and porosity of the structure are functions of solvent composition. Whereas PS fabricated from an aqueous electrolyte consists of highTable I. Summary of in situ and ex situ experiments. PS Sample
in... Aithydrous HF/MOCN rich solution MCCN/HF
(Addition) intemity Etch
Comments Figs.rr 4).)
Sun also Figures
Sigmtcusit stabilization Ralu of iocreasr/ decrease with
Etch curroni density
Figure 5(b) Figure 5(a)
Swall change but iticresan
mccl Icc HnO 2cc solution
Spectea show genes do,n.n.aen
E.haaootowsi of FL in sun
(sOn alan Pigeon 7)
lost few minutes
MeCN)HF 12cc) +
Eaiance..eat of Ft sir
(san also Pigeon 7)
_______ Comparable to
water - etch HF (-20%) in
ofF (-50%) in MeOX-etch HF (20%) in
Fsstee flue aed decay thaa HF)1150 - Pigeon 4(c) - Etch cycle behavior Pigores 8.9.
rIP (20%) in HcO
HF (20%) in HsO
Stahi)inatson of emission
Iwoot denpoff and thee slight rscnnei — not
long gnstaaon penod foe FL
— Fiss 4(d). 10 bocteo.so in Pt
Oeiset of elecmropolisbing
tsp *030 etA/crot
Dropoff in Pt
cnesidne.hly (Ref. 5) Sswpk ha. sheeter Itfesone
often footer nine in intensity —
sentsg effect Quenches
Pt is less t.tcMe in ,ubmqarnt etches - Firm 17 MeOH sad HF is
Elch with added EtOK
See Figures (4(u), 4(b). (5
Rapid non ecrntoolly plateaus
Son Figure 5
Slow rise eventually pluicous
Ittenotly increases to
_________ HP cosicenleased
(40% by volume)
cnnnibiealinn act to quench PL
(Fig (3) HF (20%) in HnO.
Stabilization st lower photon
FL level of nlrodaction 8sF (20%) in HiO
Reverse etch cunrtnn pwlunty
Oncresae of intensity and
Juralion of Pt
the surface are consistent with the formation of emitting, constrained surface species. As the open structure of PS prepared by nonaqueous etching results from an oxidastrained emitting species may also be formed on the walls of the macroporous structure and that the oxyhydrides27'28 may play an important role.
Quantum confinement vs. surface-based chemical change—As the morphology of PS depends on etching conditions,33 and the morphological changes appear to parallel changes in PL intensity,34 the source of the observed PL has been linked to a physical change in the silicon microstructure. Quantum confinement suggests that the PL originates
from nanosize particles of silicon formed during the EC
etching cycle.'182° Silicon particles with diameters less than 50 A have been reported.35 Further, correlations of the wavelength of maximum luminescence with porosity36 also suggest the possibility of size confinement and nanocrystalline silicon particles37-39 produced by techniques other than EC etching have exhibited properties similar to porous silicon.38
While enticing, the quantum confinement hypothesis is
plateau - Izior Methanol Methanol
than 100 nm of silicon need to be removed before the luminescence centers are formed. The topographical changes in
tion-dissolution process, small quantities of water are required for the onset of PL. This suggests that con-
and then rebound to
slightly higher MeCS1/HF
ly nanoporous branched structures, PS fabricated from a nonaqueous electrolyte on p-type silicon in the absence of light (required for n-type silicon) is comprised of open and accessible macroporous structures with deep, wide, and well-ordered channels.32 Random nanopores, with potentially far less accessible photoluminescent PS structures are generally formed in the aqueous etching process. Emission from the nonaqueous etched material establishes that very fine nanoporous structures are not a prerequisite to induce PL in PS. In fact, we have observed PL from both aqueous and nonaqueous etched samples prior to the formation of any pores.'2 We find that much less
Pigeon (4(a) Addition of MaCI before peaking of P1 in methanol Figure (6(o) Addi005 of M.d oboe peaking of FL in niedtantnl
!re 16(b) I4gorc 18
challenged by other experimental observations. For example, size confinement cannot account for the observed red shifts as a function of etch time (see Fig. 9) which are monitored upon the drying of the PS sample and under some oxidative conditions.4° In these experiments, the size of surface silicon particles must become smaller yet, counter to the expected manifestation of this behavior, a red shift in the PL is observed. Further, chemical change must be occur-
ring which contributes, at least heavily to (dominantly influences) the observed behavior.
Recent studies of the PL emission as a function of excitation energy in our laboratory indicate that for a selection of laser excitations over the wavelength range extending from 193 to 400 nm,9 an almost identical time-dependent
J Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemical Society, Inc.
PL emission feature results. This behavior is inconsistent with quantum confinement and suggests the pumping of the excited state manifold of a molecule-like species, followed by rapid, nonradiative relaxation through the excited state vibrational manifold and the subsequent emission of radiation at much longer wavelength emanating from considerably lower excited state levels. Our studies of the FL emission as a function of excitation
energy support the conclusions of Kanemitsu et al.,41 Frokes et al.,2'3° and Macauley et al.42 Collectively, these studies demonstrate that no obvious relationship exists between the PL spectrum and either the PLE spectrum or the particle size distribution. Kanemitsu et aL4' have used opti-
cal absorption, Raman spectroscopy, and transmission electron microscopy to assess the relationship between particle size and PL. They found a blue shift in the optical absorption spectrum for particles decreasing in size from 9 to 2 nm but observed no change in the corresponding FL peak
energy. This result clearly demonstrates that the PL peak emission energy is not correlated with particle size. Our time-dependent studies, over the 0—100 p.s time frame,9 suggest the manifestation of a pumping sequence between the ground state and strongly shifted excited state5'9 of a surface-bound fluorophor as the pumped excited state levels, high in the excited state manifold, subsequently un-
dergo rapid nonradiative relaxation. Thus, a cascade
process can lead to a red shift of the PL emission spectrum as a function of time following optical excitation at much shorter wavelength.43 This in turn suggests9 that the emission observed over a 0—100 p.s time gate may not represent
that from the lowest vibrational—rotational levels of the strongly shifted excited state. With this caveat we also establish that the time-dependent evolution of the FL in air is quite similar regardless of the manner in which a sample is prepared. The combination of these studies, in concert with the work of Prokes et al.2'2° and Macauley et al,,42 pro-
vide strong evidence suggesting that a quantum confinement process does not represent the dominant source of the observed room temperature FS FL. A number of researchers have recorded a blue shift in the PS photoluminescent emission spectrum that parallels increasing etch effectiveness. They have attributed this behavior to the creation of quantum confined silicon particulates which decrease in size with increasing etch time. However, one might also attribute the observed changes to the role of surface curvature (tension) and structural strain as it influ-
ences the PL process by creating local force gradients. In fact, Unagami44 has measured the intrinsic stress in porous silicon layers formed in an aqueous HF etch, finding a macroscopic stress which extends from compressive to tensile. Friedersdorf et al.45 have observed the influence of stress on the FL of PS structures, correlating the blue shift in PL peak energy with surface microstructure, and concluding that the characteristic cellular structure occurring in high-porosity films is due to high surface stresses. This cellular structure is not formed during the etching process itself but occurs during electrolyte evaporation after removal of the FS from solution. Enhanced surface tensions associated with increased curvature appear to be operative. Finally, in close agreement, Kanecko et al.46 have very recently noted that while an enhanced etching cycle leads to a blue shift in the PL spectrum, the higher porosity structure created is clearly strained. While these authors note that the
observed blue shift suggests quantum effects, the surface state of the porous layer also is suggested to play an important role. The changes observed in the FL emission spectra depicted in Fig. 3 and 10 as a function of etch solution can also be readily attributed to similar surface-based effects. Finally, we note that Kanemitsu et al.41" provide some indication that the FL intensity does increase significantly with decreasing particle size. This trend, which might be expected on the basis of quantum confinement,47 might also be explained by a decrease in the PL intensity resulting from an increase in the energy transfer quenchingwith increased effective particle size to which an emitting sur-
face-bound fluorophor is bound. Further, it might be
argued that the PS samples generated in anhydrous media are possessed of distinctly different effective structural sizes, suggesting that differences in the PL intensity for those samples prepared in aqueous and anhydrous media are not due entirely to surface chemical changes but to significant changes in the absorption process. However, it can also be argued that the microstructure of the PS samples generated in anhydrous media is accompanied by a signif-
icant surface roughening which can create confined regions and which results, in part, from the presence of small quantities of water which enhances the FL. Further,
it would also be surprising to find that a significant
change in the absorption process does not produce a substantial change in the spectral distribution of the FL. The characteristics which we observe as a function of etch conditions and the outlined discrepancies with the quantum confinement model naturally cause us to consider the possibility that the source of the FL is chemical in origin and surface localized. Here, the diversity of behaviors which we observe as a function of etch solution and the extremely rapid quenching of the PL which can be induced by NaF (Fig. 14) through dissolution and HI8 by rapid heavy ion quenching are certainly also suggestive of a chemistry dominated by interactions at the silicon surface—etch solution interface.
The triplet exciton emission which characterizes porous silicon has been equated to the very similar emission spectrum of "annealed" siloxene.22 However; this is a very complex species whose synthesis is tedious.23-25 Other researchers48 have shown that the luminescence is affected by the silicon hydride and silicon oxide coverage of the surface. These observations, while seemingly counter to each other, suggest that the oxygen and hydrogen functionality
on the silicon surface is important to the luminescence process. We suggest that the surface functionality of "annealed" siloxene is best described as resulting from the silicon oxyhydrides.
A chemical link.—The idea that a surface-confined moiety is the source of luminescence fits well with the FL data obtained in the initial stages and throughout the process of etching. The oxidation, complexation, and dissolution of
silicon as it transforms from the zero valent state to the fully complexed, tetravalent state (either in the solution soluble or insoluble form) proceeds through a series of electron-transfer and chemical reactions. These electrontransfer and chemical reactions should occur sequentially, the rate of each being dependent upon the chemical environment, temperature, and electrochemical potential (in the case of electron transfer). An appropriate reaction sequence involving two intermediate (metastable) states, A and B, can be represented by the following pathways
+y1H + z1X
A—x2e —- B
The exact chemical nature and rate of reaction of A and
B is dependent on the activity of the chemical species available where X can represent a variety of ligands, including F, HF, H20, OH, and oxygen. The formal oxidation state of species A and B must vary between zero and four. The species A and B might be viewed as different luminescent centers. The effect of the different electrolytes
and the experimentally generated potentials (i.e., current density) is to change the rate of formation and reaction of A and B.
For example, in the aqueous solutions, a high concentration of H30 is available which competes with F and
HF in complexing the oxidized forms of silicon. At higher fluoride concentrations, or under anhydrous conditions, the fluoride form of the silicon complex is favored as compared to the oxide or hydroxide. While it is impossible to quantitatively determine the intermediates and their rate
constants from the results in this study, the sequential
J. Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemical Society, Inc.
nature of the monitored reaction paths can be used as a framework for understanding the role of complexing agents and potential. The initial rise of the green and orange-red FL within the first minutes of etching must occur concurrently with the roughening of the surface and the formation of reaction intermediates at the silicon—solution interface. While on a short time scale the surface roughening may lead to
the formation of surface topological features consistent with quantum confinement, the formation and dissolution of unique chemical species is also possible. We contend that the most likely chemical entity which is the source of luminescence is a silicon oxyhydride.5'9 The rise in FL intensity with etch time for the basic solutions considered in this study (e.g., Fig. 4) parallels the expected increase in surface coverage of silicon reaction intermediates, possibly suboxides. Fourier transform infrared (FTIR) studies'°
show that during and after the electrochemical etching reaction, suboxides in the form of Si(II) are indeed formed
at the silicon surface. After the etching current has been terminated, any silicon dioxide and, to a slightly lesser extent, silicon-based suboxide species, formed during the etching process, should be dissolved chemically by the HF solution. Because oxide dissolution is expected to occur as the FL decays in time, the behavior of the luminescence shortly after the EC etch termination (Fig. 4) suggests that the luminescence is associated with the presence of some form of silicon oxyhydride on the FS surface. The complete oxidation of the FS surface to Si02 results in a loss of the green and orange-red luminescence. Si02 fluoresces on a much shorter time scale49 in the region near
4500 A and thus cannot be the source of the emission. In fact, the results obtained by Henglein et al.,56'51 in their study of luminescent colloidal silicon particles prepared from oxide-coated crystalline silicon formed in the combustion of silane, are relevant to our discussion. Henglein et al. found that the orange-red FL can be activated by the aqueous HF etching of colloidal silicon particles suspended in a 1:1 cyclohexane—propanol-2 solution in the presence of
air. In contrast, there is no luminescence in the absence of air (under argon). The required presence of oxygen (or small concentrations of water) indicates that the oxide layer created in the combustion of silane does not promote luminescence. Rather, as Heinglein et al. note, the development of the orange-red FL in nonpolar cyclohexane suggests that this original oxide layer must first be removed by HE The silicon particles, with a nonpolar surface, are created in the cyclohexane phase. Here an equilibrium is established between their surface oxidation and reduction by 02 (H20) and HF, respectively. Near-pristine colloidal particles are formed whose oxidation, to a much lower level than the original oxide-coated particles, produces the luminescence in a process which must compete with an eventual dissolution through SiF4 (Si(OH)4) formation.7'3252'53
Based upon a study5° of the quenching of the luminescence in polar solvents, trimethylamine, ammonia, and sulfuric acid and the apparent stabilizing effects of nonpolar solvents,7'32 Henglein et al.6° have suggested the importance of a protolytic equilibria between the three surface structures
observed decays as a function of etch solution (Fig. 4,5,8) and the fast quenching of the FL due to the introduction of NaF and HI9 to the etching solution. If the source of the
FL is a hydrogen-passivated nanocrystalline solid, one would expect only a minimal decay of the FL in the etch solution as HF only chemically dissolves silicon oxides and not silicon hydrides. As it has been demonstrated54 that the surface of fabricated porous silicon is mostly hydride-coated, consisting of (111) faces, the probability that any nanoparticles on the surface are hydride-coated is high. HF solutions react primarily with silicon—oxygen bonds to dissolve oxides. Therefore, those silicon nanopartides terminated with hydrogen should be only minimally affected by the HF solution. Further, any nanocrystalline silicon particle terminated by an oxide coating would be expected to decrease in size as the dissolution process concludes with a hydride surface termination. As a result, a slight decay in FL and not the complete elimination of FL
would be expected if the FL was associated with nanocrystalline surface structures. The luminescence decays depicted in Fig. 4 and 5 can also be demonstrated to be consistent with a surface-confined moiety as the source of the FS PL.5'7'9 A plausible explanation for the growth and decay of the green and orange-red FL is based upon the formation and oxidative chemical transformation of the silicon oxyhydrides.5 Experimental observations of the time-dependent behavior of the in situ FL depicted in Fig. 4b and c combined with the quantum chemical modeling of the low-lying electronic states of the silanone-based silicon oxyhydrides7'6 provides strong support for the hypothesis that the long-lived green FL5 and its subsequent transformation to a final orange-red emission are associated with the chemical transformation of surface-bound oxyhydrides. The details of our modeling study have been given elsewhere,5'926 however, the most relevant results are presented for the silanone-based silicon oxyhydrides in Tables II
and III. Further calculations were also carried out on the ground and lowest lying electronic states of the silylenes and dangling electron SiXYZ compounds which vary through the series from SiH2 to Si(OH)2. In Table II we
summarize the SiO bond lengths calculated at the MF2/DZF5'26 level for the ground state singlets and lowest lying excited state triplets of several model silanone-based oxyhydride compounds which we have considered.6'9'26 The
calculations on the SiXYZ compounds from SiH2 to Si(OH)2 26 demonstrate that these molecules possess excited states whose lowest lying transitions all lie far into the
ultraviolet region and are therefore inaccessible to the light sources used in this study. The calculations on the silanones demonstrate a significant change accompanying the transition to a low-lying excited triplet state which produces a considerable lengthening of the SlO bond.66'56 In contrast, calculations on the corresponding silylene isomers demonstrate much smaller changes in the bond lengths and bond angles of the low-
Table II. Si=O bond lengths (A) for silanones at the MP2/DZP level.
Fast quenching and quantum confinement—The quan-
tum confinement theory is not consistent with the
with the neutral hydroxyl structure corresponding to that species which can be expected to produce the orange-red
luminescence. Thus, these authors suggest that the orange-red FL occurs when colloidal silicon particles carry only a limited component of oxidized centers and
that the protonation state of these centers strongly affects the luminescence. This result is quite consistent with the formation of a silicon oxyhydride constituency encompassing a required OH or OR ligand.
Si(O)H2 Si(O)H(OH)6 Si(O)(OHl2 Si(O)H(OS1H2) Si(O)SiH3(OSiH3l Si(Ol(OSjH3)2 Si(O)H(SiH3l Si(O)(OH)(SiH2) Si(O)(SiH5)5
1.545 1.537 1.536 1.537 1.543 1.537 1.553 1.543 1.560
1.709 1.709 1.708 1.712 1.704 1.695 1.712 1.681
a Bond length for the excited singlet ii 1.705 A.
Ar(SiO) 0.155 0.172 0.173 0.171 0.169 0.167 0.142 0.169 0.121
Bond lengths for HO—Si—QH silylene are 1.670 A for the ground-state iinglet and 1.680 A for the exciied triplet.
J. Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemical Society, Inc.
Table Ill. Ground-state singlet—excited energy separation for silanones (silylenes).
60.1 70.9 71 70.3 69.6 67.1 71.2 57.3 53.9 38.4 64.2
475 403 402 406 411 426 401
Si(O)H5 Si(O)H(OH) Si(O)(OH)2
Si(rnH(0S1H5) Si(O)SiH5(OSiH9) Si(O)(OSiH3)5 Si(O)(OH)(S1H5)
HSiOH HOSiOH SiH3OSiOH
3.07 3.08 3.05 3.02 2.91 3.09 2.48 2.34 1.66 2.78 2.92
499 530 744 445 425
lying excited states which can he accessed via excitation spectroscopy in the appropriate spectral regions. The data in Table III indicate the calculated singlet-triplet separations for the model compounds of interest. It is noteworthy that the calculated locations of the silanone-based silicon oxyhydride excited triplet states for Si(O)H(OH), Si(O)(OH)5, Si(O)H(OSiH5), Si(O)SiH5(OSiH5), and Si(O)OH(SiH5) con-
taining an OH or OSiH5 moiety and the known peak wavelength of the porous silicon excitation spectrum (—350 nm)29 bear a clear resemblance to the known singlet-triplet splittings of the low-lying silicon monoxide intercombination band systems.55 The large change in the SiO bond lengths indicated in Table II for all the silanones in turn produces a
large shift in the excited state potentials relative to the ground state. The relative location of the ground and excited state potentials, especially for the OH— or OSiH5—bonded
silanones, promotes optical pumping high up the excited state potential and a significant difference in the peak of the PLE spectrum (—350 nm) and the observed PL emission range [—500—550 nm (green), —600—800 nm (orange)]. While
the experimental data are consistent with a most efficient excitation pumping high up the excited triplet state mani-
silanones with only -R group ligands. Excitation of these latter silanones should be more efficient at longer wavelengths, consistent with the experimental observations of a strong green in situ PL for Hg lamp vs. KrF and ArF optical pumping. It is also to be noted that the unsaturated bonding which we consider would appear necessary in order that the electronic transitions of interest for these Si, 0, and H compounds fall within the visible and UV regions. The green—to—orange-red PL transformation —The
sources of the "orange-red" PL emission which corre-
spond to -Si(O)OH or -Si(O)OR constituencies would be expected to undergo dissolution at a more rapid rate than the -H or -R (vs. -OH or -OR) group terminated oxyhydrides. This certainly follows the experimentally observed very long time decay of the PL which can be followed visually to observe that the "orange-red" PL will first decay completely followed by the subsequent loss of any residual "green" PL emission. The green and orange-red emissions have been previously assigned to interlocking exciton fluorescence and phosphorescence emissions, respectively.19 The experimental data," however, favor a chemical transformation process involving two distinct surface species whose photogenerated excited states have comparable emission lifetimes.' Although the overlap of the spectral features associated with the green and orange-red emitters prevents a ready evaluation of the radiative lifetime associated with the green emitter, its radiative decay routes do not appear to be compatible with a fast fluorescence process and are far
less rapid than that of the short-lived Si05 emission at 450 nm,49 Our observations suggest a chemical conversion
between two moderately long-lived (several microsec-
onds)5'9 surface-bound constituencies and establish that an intersystem crossing process involving a short-lived green and long-lived orange emitter, as suggested by others,1925 seems far less likely Based on the results of our quantum mechanical modeling, we assign the green and orange-red
dence for subsequent rapid nonradiative vibrational relax-
emissions to the silanone-based oxyhydrides in various stages of oxidation.9 The growth of the FL with time during and for some period after the etch cycle is consistent with an increasing surface coverage of the FL emitters as
emission9'26 of radiation.
their formation competes with dissolution.9'12 As the oxide dissolution occurs and the FL decays in time, the oxidized
fold5'9 for these silanone-based compounds, there also is evi-
ation through this excited state manifold before the There are additional striking aspects to the data in
Tables II and iii. First, from Table II we note that whenever an OH or OSiH5 group (Table II, lines 2, 4, 5, and 8)is bound to the silicon—oxygen bond, the calculated change, 4r
(SiO), in transition is consistently a substantial 0.17 A.
Further, an additional OH group does little to affect this differential change in the bond length accompanying the sin-
glet—triplet transition. In the absence of an -OH or -OR
group, the change is notably smaller, decreasing from 0.155 A for Si(O)H5 to 0.121 A for Si(O)(S1H5). These are distinct differences associated with -OR vs. -R group bonding to the silicon which can have a considerable affect on the relative energies of PLE excitation and PL emission spectra. Further, we note the very similar adiabatic energy differences (AE 3.05 e11) which characterize those singlet—triplet transitions where an -OH or -OR group is bound to the silicon oxide bond. The shift of the excited triplet state relative to
the ground state singlet suggests that a peak maximum at —3.5 eV should be observed in the PLE excitation spectrum
associated with a silanone-based oxyhydride emitter containing an -OH or -OR group. While the virtually identical energy increments for those silanones containing an -OR
group can be contrasted with the much lower required
pumping energies associated with the series Si(O)H2 (0.155), Si(O)H(SiH5) (0.142), and Si(O)(SiH5)2 (0.121), these latter silanones display a smaller change, Ar (SiO), in the SiO bond
length, which is expected to lead to a considerably smaller
red shift of the PL emission feature relative to the PLE wavelength.5
The results of the outlined quantum chemical modeling suggest that the unsaturated silanones with bound -OR hgands produce a much larger red shift of the PL emission spectrum relative to the peak of the PLE spectrum than will
silanone-based oxyhydrides terminated with -OH or -OR groups (the orange-red emitters) undergo dissolution at a more rapid rate than those -H or -R group terminated oxyhydrides (the green emitters)." Current density dependence and the silicon suboxides.— Current density also plays an important role in the etching process. With the aqueous HF etching solutions, two etching regimes exist and are defined by a critical current denAt j > j,, electropolishing of the silicon sursity face occurs. At j < j,,, pores are formed. At low current densities the electro-oxidation reaction ultimately results in dissolution of SiF4, whereas at high current densities dissolution occurs by formation of both S1F4 and S102 or Si(OH)4. Even at low current densities, the reaction of silicon with water (producing surface hydroxyl groups) is significant. We have argued7 that the formation of hydroxyl groups on the surface facilitates the formation of photoluminescence centers. Two reactive modes of water with the silicon surface can be envisioned: (i) the formation of silicon hydride and silicon hydroxide bonds across adjacent silicon surface atoms (Fig. 17), and (ii) the concerted reaction of a water molecule at a silicon atom site to form the oxide,'° with the subsequent release of hydrogen or the a The evaluation of a radiative lifetime for the green-emitting precursor state can be complicated both by its continual formation and by its chemical transformation during the course of an emission decay measurement. Reports of enhanced orange—red FL emission after RTDO
where the OH content is believed minimal might be deemed ioconsistent with a surface-bound silanone structure. However,
Yan et al.28 have certainly obtained evidence that ressdual hydrogen exists in a thermally oxidized PS film, probably in the form of SiOH.
J Electrochem. Soc., Vol. 145, No. 9, September 1998 The Electrochemical Society, Inc.
insertion of the oxygen into a silicon—silicon surface bond. At j